Synthesis, characterization, thermal and electrochemical
properties of imine polymers containing pyridine and
Hatice Karaer1), 2), İsmet Kaya1), *), Haluk Aydın2)
Abstract: Schiff bases polymers were synthesized from 2-hydroxybenzaldehyde (2-HBA) via oxidative polymerization method in an aqueous alkaline medium in the presence of NaOCl as an oxidant. Then, these polymeric Schiff bases were prepared from the polyaldehyde by grafting each of them with dif-ferent amines containing pyridine and pyrimidine groups. The structures of polymers were confirmed by FT-IR, 1H NMR, 13C NMR, and UV-Vis measurements. The polymers were characterized by GPC and SEM analyses. Furthermore, their optical properties were determined by UV-Vis and fluorescence spec-troscopy, their electrochemical properties by cyclic voltammetry (CV) analysis and solid state conduc-tivity measurements by the four-point probe technique, their thermal behavior by TG, DTA, and DSC measurements. The electrical conductivity of the polymers was also measured and found that they are semiconductive. The number average molecular weight (Mn), the weight average molecular weight (Mw), and dispersity (Đ) values of the polymers were found from GPC analysis and were equal 5900, 5450 and 1.08, respectively, for poly(2-hydroxybenzaldehyde) (P-2HBA) polymer. Electrochemical energy gap (E’g) was found by CV, whereas optical band gap (Eg) was determined by UV-Vis measurements.
Keywords: poly(imines), poly(phenoxy-imines), optical properties, thermogravimetric analysis, semi-conductivity.
Synteza, charakterystyka, właściwości termiczne i elektrochemiczne
polime-rów iminowych zawierających jednostki pirydynowe i pirymidynowe
Streszczenie: Polizasady Schiffa zsyntetyzowano metodą polimeryzacji utleniającej 2-hydroksybenzal-dehydu (2-HBA) w środowisku alkalicznym, w obecności NaOCl jako utleniacza, a następnie szcze-piono otrzymany polialdehyd za pomocą amin zawierających grupy pirydynowe i pirymidynowe. Uzyskane polimery charakteryzowano metodami GPC i SEM, a ich struktury potwierdzono za po-mocą spektroskopii FT-IR, 1H NMR, 13C NMR i UV-Vis. Właściwości optyczne polizasad Schiffa ana-lizowano spektroskopią fluorescencyjną i UV-Vis, a właściwości termiczne określono metodami TG, DTA i DSC. Korzystając z woltamperometrii cyklicznej (CV) oraz pomiarów przewodności ciała stałego metodą czteropunktową badano właściwości elektrochemiczne otrzymanych polimerów. Pomiary te wskazują na półprzewodnikowy charakter polimerów. Stwierdzono, że wartości liczbowo średniego ciężaru cząsteczkowego (Mn), wagowo średniego ciężaru cząsteczkowego (Mw) i stopnia polidyspersji (Đ) poli(2-hydroksybenzaldehydu) (P-2HBA) wyznaczone na podstawie analizy GPC są równe, odpo-wiednio, 5900, 5450 oraz 1,08. Szerokość elektrochemicznej przerwy energetycznej (E’g) oznaczono me-todą CV, natomiast szerokość optycznej przerwy energetycznej (Eg) za pomocą spektroskopii UV-Vis. Słowa kluczowe: poli(iminy), poli(fenoksy-iminy), właściwości optyczne, analiza termograwimetrycz-na, półprzewodnictwo.
Polymeric Schiff bases (polyimines or
polyazome-thines) are a class of materials containing the -CH=N- structural unit that exhibit good thermal stability and ad-vantageous mechanical properties . Polymeric Schiff bases generally show basic properties, since they have a C=N linkage in backbone. Considerable interest has been focused on this polymers due to their thermal stability, potential semiconductivity, conductivity, and non-linear optical properties . Polyazomethines (PAMs) possess-ing p-conjugated systems have low band gaps and,
con-1) Çanakkale Onsekiz Mart University, Faculty of Sciences
and Arts, Department of Chemistry, 17020, Çanakkale, Turkey.
2) Dicle University, Faculty of Science, Department of
Chemi-stry, 21280, Diyarbakır, Turkey.
sequently, are semiconductive . They were synthesized by polycondensation of dialdehydes or diketones with an aliphatic or aromatic diamine to give high molecu-lar weight polymers . Polyimines including conjugated bonding and active hydroxyl group have been studied for more than 60 years and have been used in various fields owing to their useful properties such as paramagnetism, semiconductivity, electrochemical cell, and resistivity to high energy. They are used to prepare composites with high positive temperature coefficient of resistance, ther-mostabilisators, graphite materials, epoxy oligomer and block copolymers, and photo resists as well as photo ma-terials, which are antistatic and enduring to flame . Schiff base substituted oligophenol derivatives are usu-ally synthesized by oxidative polycondensation reaction of the corresponding Schiff base using cheap oxidants such as H2O2, NaOCl, and air . The main advantage of the oxidative polycondensation method is the usage of easily available, simple and cheap structured oxidants . Oxidative polymerization is one of the important green chemistry processes to prepare multifunctional polymers, and widely used to prepare different types of polymers such as polyaniline, polythiophene, polyfluo-rene, polypyrrole, polyphenol, polycarbazole, poly Schiff bases, and their different derivatives .
In this study, the oxidative polycondensation reactions of 2-hydroxybenzaldehyde, were studied by using NaOCl oxidant in an aqueous alkaline medium at 70 °C. Then, poly Schiff bases were prepared from the polyaldehyde by grafting each of them with six different amines contain-ing pyridine and pyrimidine groups. The structures of the synthesized polymers were approved by FT-IR, 1H NMR, 13C NMR spectroscopy, GPC and SEM analyses, UV-Vis and fluorescence spectroscopy, CV analysis, solid state conductivity measurements, and by TG-DTA analysis.
EXPERIMENTAL PART Materials
2-Hydroxybenzaldehyde (2-HBA), ethanol, KOH, and HCl were supplied by Merck Chemical Co. (Germany) and used as received. Sodium hypochlorite (30 % aqueous solution of NaOCl) was purchased by Paksoy Chemical Co. (Turkey). 2-Amino-3-methylpyridine (3MP), 2-ami-no-6-methylpyridine (6MP), 2-amino-4-methylpyridine (4MP), 2-amino-4,6-dimethylpyrimidine (46MP), 2,4,6-tri-aminopyrimidine (TAP), 2-2,4,6-tri-aminopyrimidine (2AP) were supplied from Sigma-Aldrich and they used as received. Synthesis of P-2HBA with NaOCl in an aqueous alkaline medium
P-2HBA was synthesized through oxidative polycon-densation of 2-HBA with an aqueous solution of NaOCl (30 %) as in the literature [8–11]. 2-HBA (0.001 mol) was dissolved in an aqueous solution of KOH (0.001 mol, 10 %)
and placed into a 100 cm3 three-necked round-bottom flask. It was fitted with a condenser, thermometer, stirrer, and an addition funnel containing NaOCl. After heating it to 70 °C, NaOCl was added dropwise for almost 30 min. The reaction mixture was cooled to room temperature, and then 0.001 mol HCl (37 %) was added to solution. The crude product was washed with 25 cm3 of hot water for three times for the separation from mineral salt. Synthe-sis reaction, resonance forms and combination of radicals, and structure of P-2HBA are shown in Schemes A–C, re-spectively.
Synthesis of Schiff base polymers
The poly Schiff bases abbreviated as P-2HBA2AP, P-2HBA46MP, P-2HBATAP, P-2HBA3MP, P-2HBA4MP and P-2HBA6MP were synthesized by the condensa-tion reaccondensa-tion of 2-aminopyrimidine (2AP), 2-amino-4,6--dimethylpyrimidine (46MP), 2,4,6-triaminopyrimidine (TAP), 2-amino-3-methylpyridine (3MP), 2-amino- -4-methylpyridine (4MP), and 2-amino-6-methylpyridine (6MP) with poly(2-hydroxybenzaldehyde), respectively
HO CHO + NaOH + H2O NaO CHO + + -NaO CHO + NaOCl •O CHO + 2 OH- + 2 NaOH O• CHO O CHO • O CHO • 2 • O CHO OHC O O CHO • O CHO + • O CHO O OHC O CHO HO OHC OH OH CHO CHO CHO HO HO OHC
(Scheme D). Poly(2-hydroxybenzaldehyde) was weighed and put into a 100 cm3 three-neck, round bottom reac-tion flask separately, and then 30 cm3 of methanol was added and it was dissolved at room temperature by con-tinuous mixing on a hot plate magnetic stirrer under condenser. Then, amines, 3MP (1.08 g, 1 x 10-2 mol), 6MP (1.08 g, 1 x 10-2 mol), 4MP (1.08 g, 1 x 10-2 mol), 46MP (1.2 g, 1 x 10-2 mol), TAP (1.25 g, 1 x 10-2 mol), and 2AP (0.95 g, 1 x 10-2 mol) dissolved in 10 cm3 of methanol were added into the reaction flask, and were left to form a poly Schiff base monomer at 70 °C . Dark brown-black polymers were obtained at the end of the reaction.
Methods of testing
The infrared and ultraviolet–visible spectra were re-corded by a PerkinElmer FT-IR Spectrum one and Analy-tikjena Specord 210 Plus, respectively. The FT-IR spectra were recorded using a universal ATR sampling accessory
(4000–550 cm-1). 1H and 13C NMR spectra were performed using Bruker AV400 spectrometer (T = 25 °C, solvent – deuterated DMSO-d6, internal standard – tetramethylsi-lane). Thermal data were obtained using a PerkinElmer Diamond Thermal Analysis system. TG–DTA measure-ments were made under a nitrogen flow and at a heating rate of 10 °C/min from room temperature to 1000 °C. DSC analyses were carried out using a PerkinElmer Pyris Sap-phire DSC. DSC measurements were made in the range 25–450 °C (in N2, heating rate 10 °C/min). The number average molecular weight (Mn), weight average molecu-lar weight (Mw), and dispersity (Đ = Mw/Mn) were deter-mined by Gel Permeation Chromatography-Light Scat-tering (GPC-LS) device of Malvern Viscotek GPC Dual 270 max. GPC-LS analyses were performed at 55 °C using DMF with lithium bromide (1 g/dm3) as eluent at a flow rate of 1 cm3/min. A medium 300 x 8.00 mm dual column was used. A refractive index detector (RID), Light Scatter-ing Detector (LS), and polystyrene standards were used N N NH2 N N H2N N N H2N NH2 NH2 N H2N N H2N N H2N P-2HBA i i i i i i OH C H N N N P-2HBA46MP OH CHO NaOCl
KOH(aq.), 70 °C CHO
OH 2-HBA P-2HBA N N CH OH N N N CH HO N N C HO H N N CH HO N N N HC OH HC OH P-2HBATAP P-2HBA4M P C H N N OH P-2HBA6MP i: Ethanol, 24 h70 °C P-2HBA3M P P-2HBA2A P Scheme D
to analyze the products. Surface morphology of the poly-mers was determined by field emission scanning elec-tron microscope (FE-SEM, JEOL, JSM-7100). Conductivity was measured by a Keithley 2400 Electrometer (Keithley, Ohio, USA). The pellets were pressed on hydraulic press at 1687.2 kg/cm2. Iodine doping was performed by ex-posing the pellets to iodine vapor at atmospheric pres-sure and room temperature in a desiccator . Cyclic voltammetry (CV) measurements were performed by a CHI 660C Electrochemical Analyzer (CH Instruments, Texas, USA) at a potential scan rate of 20 mV/s. All ex-periments were carried out in a dry box filled with ar-gon at room temperature. The electrochemical potential of Ag was calibrated with respect to the ferrocene/ferro-cenium (Fc/Fc+) couple. The half-wave potential (E1/2) of (Fc/Fc+) measured in 0.1 M tetrabutylammonium hexa-fluorophosphate (TBAPF6) acetonitrile solution is 0.39 V with respect to Ag wire. The voltammetric measurements were performed in acetonitrile . An ultrasonic bath was used to dissolve the samples. The HOMO–LUMO energy levels and electrochemical band gaps (E’g) were calculated from the reduction and oxidation peak poten-tial and onset values. The UV-Vis spectra were recorded using MeOH as a solvent, at 25 °C. The optical band gaps (Eg) were calculated from their absorption edges .
RESULTS AND DISCUSSION Structures of the compounds
The FT-IR spectrum of P-2HBA polymer was not signif-icantly different from that of the 2-HBA monomer, as ex-pected. FT-IR spectra of P-2HBA and 2-HBA are given in Fig. 1. However, peaks of P-2HBA polymer were broader than that of 2-HBA monomer after the polycondensation reaction owing to their polyconjugated structures. More-over, the edged peaks of 2-HBA monomer were broad-er and decreased numbroad-erically because of the increase in molecular weight after polymerization reactions , confirming polymerization of 2-HBA. Bands in the FT-IR
spectra of the polymers decreased due to their conjugated bond systems .
As seen in Fig. 1, -OH stretching band was observed at 3320 cm-1, aromatic -CH peak at 3060 cm-1, aldehyde -CH peak at 2847 cm-1 for P-2HBA polymer. The peak at 1658 cm-1 corresponds to -C=O stretching vibration of al-dehyde for P-2HBA. Furthermore, peaks at 1450–1650 cm-1 were assigned to benzene cycle and C=C moiety and those at 1000–1400 cm-1 were attributed to C-O stretching . Again, those at 1578 and 1481 cm-1 correspond to aromatic C=C and those at 1273 cm-1 were due to C-O bending vi-bration peaks for phenol group. Peaks of P-2HBA were broader than those of 2-HBA, implying that 2-HBA polym-erized . The broad peak at about 3500–3000 cm-1 corre-sponds to hydroxyl -OH stretching. Additionally, aromatic -CH stretchings were observed at 3000–2900 cm-1, while aliphatic ones for methyl -CH3 group were seen at 2950– –2900 cm-1 except for -TAP and -2AP coded polymers. The peak at 1608, 1602, 1610, 1629, 1610 and 1633 cm-1 corresponds to -CH=N stretching vibration of imine for P-2HBA3MP, P-2HBA4MP, P-2HBA6MP, P-2HBA46MP, P-2HBATAP and P-2HBA2AP, respectively.
As expected, in the FT-IR spectra of the poly Schiff bases, functional groups different from P-2HBA were observed, confirming formation of the polymers. In the FT-IR spectra of poly Schiff bases, pyridine and pyrimi-dine groups were given separately in Fig. 2a and Fig. 2b, -3MP, -4MP and -6MP coded materials contain pyridine groups, whereas -46MP, -TAP and -2AP coded materials include pyrimidine groups.
The structures of the poly Schiff bases were confirmed by newly appeared imine -CH=N peaks, disappearing of the amine -NH2 peaks and the C=O peaks of the aldehyde used in the condensation reactions. These changes are also shown in Fig. 2a and Fig. 2b.
1H NMR and 13C NMR data of the polymers are listed in Table 1. It is known that phenol based Schiff bases poly-merize by oxidative polymerization via C-C ortho and/or
para positions of the ring in terms of -OH or C-O-C
bind-ing via oxygen atom of -OH moiety (Scheme D). Integration ratio of the -OH proton at 10.80 ppm decreases compared to that of -CHO at 10.26 ppm, however, the signal does not completely disappear, indicating that -OH moiety does not lose, it remains after polymerization. This shows also that proton of -OH leaves and polymerization occurs via oxy-gen atom (10 %).
In the 1H NMR spectrum of the poly Schiff base, de-crease of integration ratio of the protons at ortho and para positions of the ring in terms of -OH group after polym-erization shows that these protons decrease in numbers compared to the other protons in the structure . It is understood from the decreasing in the integration of -OH that polymerization occurs through -C-O-C- bind-ing, mainly C-C binding exists and it occurs at the point where -Ha proton exists. Resonances in the 1H NMR spec-trum of the polymer broadened after oxidative polymer-ization, showing that monomers repeated in the structure. Wave number, cm-1 4000 2000 650 1149 750 1186 1273 1481 1644 1578 1658 2735 2-HBA 2847 1000 P-2HBA 3000 T ransmittance
T a b l e 1. NMR spectra data of the polymers
Polymers NMR spectra data, ppm
2 3 6 5 4 1 CHO Hd Hb Hc Ha OH 7 P-2HBA 1H NMR (DMSO-d
6, ppm, δ): 10.80 (s, -OH), 7.54 (d, Ar-Hd), 7.52 (t, Ar-Hb), 7.50 (d, Ar-Hc), 6.99 (d, Ar-Ha), 9.84 (s, -CHO).
13C NMR (DMSO-d
6, ppm, δ): 119.92 (C1-ipso), 122.72 (C2-H), 117.50 (C3-ipso), 161.03 (C4-ipso), 145.87 (C5-ipso), 129.66 (C6-H), 192.22 (C7-H),
136.78, 119.62, 116.02 (new peaks, C-O-C and C-C coupling).
2 3 4 5 6 1 OH CH N 7 N 11 10 9 8 H3C 13 12 P-2HBA3MP 1H NMR (DMSO-d
6, ppm, δ): 10.26 (s, -OH), 6.80-8.33 (m, aromatic protons), 8.13 (s, -CH=N).
13C NMR (DMSO-d
6, ppm, δ): 119.77 (C1-H), 117.09 (C2-H), 123.59 (C3-H), 116.16 (C4-H), 146.78 (C5-ipso), 145.28 (C6-ipso), 164.04 (C7-ipso), 129.38 (C8-ipso), 128.18 (C9-H),
137.42 (C10-H), 156.00 (C11-H), 161.22 (C12-H), 17.22 (C13, CH3), 133.74, 139.97, 123.69 (new peaks, C-C coupling).
P-2HBA4MP 2 3 4 5 6 1 OH CH N 7 N 11 10 9 8 CH3 13 12 1H NMR (DMSO-d
6, ppm, δ): 10.54 (s, -OH), 6.55-8.50 (m, aromatic protons), 8.22 (s, -CH=N).
13C NMR (DMSO-d
6, ppm, δ): 117.79 (C1-H), 122.54 (C2-H), 120.79 (C3-H), 136.63 (C4-H), 147.44 (C5-ipso), 157.06 (C6-ipso), 164.81 (C7-ipso), 114.35 (C8-H), 113.79 (C9-ipso),
129.63 (C10-H), 160.05 (C11-H), 161.27 (C12-H), 21.01 (-CH3), 133.61 (new peak, C-C coupling).
P-2HBA6MP 2 3 4 5 6 1 OH CH N 7 N 11 10 9 8 CH3 13 12 1H NMR (DMSO-d
6, ppm, δ): 10.53 (s, -OH), 6.50-8.00 (m, aromatic protons), 8.19 (s, -CH=N).
13C NMR (DMSO-d
6, ppm, δ): 117.24 (C1-H), 111.02 (C2-H), 119.85 (C3-H), 122.72 (C4-H), 133.67 (C5-ipso), 156.45 (C6-H), 164.41 (C7-ipso), 122.58 (C8-H), 122.58 (C9-H),
137.67 (C10-H), 159.57 (C11-ipso), 161.43 (C12-H), 24.10 (C13, -CH3), 139.17 (new peak, C-C coupling).
P-2HBA46MP 2 3 4 5 6 1 OH CH N 7 N 9 8 9 N CH3 CH3 11 10 10 1H NMR (DMSO-d
6, ppm, δ): 10.70 (s, -OH), 6.50-8.00 (m, aromatic protons), 8.17 (s, -CH=N). OH CH N N N CH CH HO HO P-3HBATAP 1H NMR (DMSO-d
6, ppm, δ): 10.20 (s, -OH), 5.50-7.55 (m, aromatic protons), 8.33 (s, -CH=N). P-2HBA2AP 2 3 4 5 6 1 OH CH N 7 N 8 9 8 N 10 1H NMR (DMSO-d
6, ppm, δ): 10.37 (s, -OH), 6.50-7.55 (m, aromatic protons), 8.42 (s, -CH=N).
13C NMR (DMSO-d
6, ppm, δ): 118.16 (C1-H), 129.66 (C2-H), 119.92 (C3-H), 122.42 (C4-H), 136.91 (C5-ipso), 158.06 (C6-ipso), 171.67 (C7-ipso),
166.48 (C8-H), 117.43 (C9-H), 163.89 (C10-H), 136.10 (new peak, C-C coupling).
Five different carbons are observed at structure of P-2HBA. In the 13C NMR spectrum, decreasing of reso-nance intensity of C6 and appearing of a new resoreso-nance at 145.87 ppm clearly indicate that phenoxy unit, which occurred from -OH group bound to C6 (ipso-carbon),
forms the polymer structure consisting of oxyphenylene units C-O-C. New signals were observed in the region of 140 to 160 ppm owing to -C-O-C- coupling, which con-firm polymerization occurred via -OH moiety .
As stated in the previous studies, phenol-based mono-mers may be polymerized either by C-O-C binding via ox-ygen atom of -OH or by C-C coupling of monomer units with ortho or para position of the phenol in terms of -OH group . The short resonances at 119.62 and 116.02 ppm obviously indicate that P-2HBA polymerizes through C1 and C3 carbons, i.e., C-C binding occurs for the radical occurred at ortho or para position of phenol by distribu-tion of the phenoxy radical to the cycle. Schemes A–C display oxidative polymerization reaction mechanism of P-2HBA. The hydroxyl, aldehyde and aromatic proton signals of P-2HBA were observed in 10.80, 9.84 and 7.54– –6.99 ppm range, respectively, in the 1H NMR spectrum. In the 13C NMR spectra, resonances for polyaldehyde C=O and hydroxyl carbon atoms are observed at 192.22 and 161.03 ppm, respectively.
In the 1H NMR spectra of poly Schiff bases, the signal of aldehyde proton (at 9.84 ppm) of P-2HBA disappears and a new signal between 8.13 and 8.42 ppm appears, indicating azomethine formation -CH=N. In the 13C NMR spectra, res-onances for poly Schiff bases -CH=N carbon atoms are ob-served between 161.22–163.89 ppm. Aliphatic -CH3 carbon signals of P-2HBA3MP, P-2HBA4MP and P-2HBA6MP were observed in 17.22, 21.01 and 24.10 ppm, respectively, while in the 1H NMR spectra, aliphatic -CH
3 protons are observed at 2.36, 2.12, 2.20 and 2.45 ppm for P-2HBA3MP, P-2HBA4MP, P-2HBA6MP and P-2HBA46MP, respectively.
According to the GPC chromatograms, the calculat-ed number average molecular weight (Mn), weight av-erage molecular weight (Mw), and dispersity (Đ) values of P-2HBA3MP, P-2HBA4MP, P-2HBA6MP, P-2HBATAP, P-2HBA46MP and P-2HBA2AP were measured by RI detector, are given in Table 2. According to these re-sults, P-2HBA, P-2HBA3MP, P-2HBA6MP, P-2HBA4MP, P-2HBA 46MP, P-2HBATAP and P-2HBA2AP contain
ap-T a b l e 2. GPC analysis results of the polymers
Molecular weight distribution parameters
Fraction I Fraction II Mw Mn Đ Mw Mn Đ % Mw Mn Đ % P-2HBA 5900 5450 1.08 – – – – – – – – P-2HBA3MP 12350 9700 1.27 – – – – – – – – P-2HBA6MP 11370 9200 1.24 – – – – – – – – P-2HBA4MP 7800 5650 1.23 18500 13400 1.38 70 8550 6300 1.36 30 P-2HBA46MP 12450 10300 1.21 – – – – – – – – P-2HBATAP 7900 5750 1.37 17900 12800 1.40 75 9650 7500 1.29 25 P-2HBA2AP 14500 11900 1.22 – – – – – – – –
Mn– number average molecular weight; Mw– weight average molecular weight; Đ – dispersity.
Wave number, cm-1 4000 2000 650 -OH 1000 3000 T ransmittance P-2HBA6MP P-2HBA3MP P-2HBA4MP -CH=N 1610 1144 1225 1451 1550 1602 1110 1151 1195 1452 1188 1226 1454 1554 1034 1562 1608 Wave number, cm-1 4000 2000 650 -OH 1000 3000 T ransmittance P-2HBA2AP P-2HBATAP P-2HBA46MP -CH=N 1633 1151 1277 1481 1586 1629 1103 1224 1454 1451 1178 1275 1453 1562 1094 1558 1610 1223
Fig. 2. FT-IR spectra of poly Schiff bases containing: a) pyridi-ne, b) pyrimidine
proximately 45–49, 46–59, 44–54, 27–37, 46–55, 13–18 and 60–73 repeated units, respectively.
Thermal analysis of the polymers
TG and DSC thermograms were taken to determine the temperatures corresponding to 20 and 50 % weight losses of the polymers (T20, T50), the initial degradation tempera-tures (Ton), the number of decomposition steps, exother-mic and endotherexother-mic peaks, glass transition tempera-tures (Tg), and specific heat change (∆Cp) of monomers. The values measured from thermograms are shown in Table 3. TGA curves of the polymers are shown in Fig. 3.
Ton of the polymers, P-2HBA, P-2HBA2AP, P-2HBA46MP, P-2HBATAP, P-2HBA3MP, P-2HBA6MP and P-2HBA4MP were found to be 139, 250, 120, 203, 145, 135 and 122 °C, respectively. T50 were calculated as 866, 866, 820, 535, 660 and 638 °C for P-2HBA, P-2HBA2AP, P-2HBATAP, P-2HBA3MP, P-2HBA6MP and P-2HBA4MP, respectively. The glass transition temperatures of the polymers lie be-tween 112 and 188 °C, as observed in DSC analysis. Ac-cording to the thermal analysis data, it can be said that the polymers are thermally stable.
Electrochemical and conductivity properties of polymers
The voltammetric measurements were performed in acetonitrile. The values of electrochemical band gaps (E’g) were given in Table 4. These data were estimated by
us-ing the oxidation onset (Eox) and reduction onset (Ered)
val-ues, as given in Fig. 4 for the polymers. The calculations were performed by using the following equations :
EHOMO = -(4.39 + Eox) (1)
ELUMO = -(4.39 + Ered) (2)
E’g = ELUMO – EHOMO (3)
The HOMO–LUMO energy levels and the electrochem-ical band gaps were also given schematelectrochem-ically in Fig. 5. It is seen that the electrochemical band and optical gaps val-ues of the polymers were changed between 2.78–2.48 eV and 2.96–2.19 eV, respectively (Table 4).
10 200 400 600 800 1000 100 50 0 Mass, % P-2HBA P-2HBA46MP P-2HBATAP P-2HBA2AP P-2HBA6MP P-2HBA4MP P-2HBA3MP Temperature,°C
T a b l e 3. Thermal degradation values of the polymers
°C T°C max T°C20 °CT50 carbine residue at 1000 °C, wt % Exo / Endo ΔCTgp, °C /, J/g·°C
P-2HBA 139 157, 860 333 866 39 805 / – 112 / 0.118 P-2HBA2AP 250 291, 873 752 866 10 306, 793 / 879 116 / 0.855 P-2HBA46MP 120 126, 335, 583 373 – 52 – / – 114 / 0.215 P-2HBATAP 203 235, 836, 913 324 820 4 318, 803 / – 188 / 0.321 P-2HBA3MP 145 151 143 535 36 – / – 123 / 0.044 P-2HBA6MP 135 148, 567, 953 170 660 21 – / – 118 / 0.163 P-2HBA4MP 122 146, 572, 803 171 638 37 594 / – 113 / 1.246
Ton – the onset temperature; Tmax – temperature of the maxima of the peaks; T20 – temperature corresponding to 20 % weight loss; T50 –
temperature corresponding to 50 % weight loss; Tg – glass transition temperature; ΔCp – change of specific heat during glass transition.
Fig. 3. TGA curves of the polymers
Potential, V -1.6 0 1.6 1.2 -0.8 P-2HBA6MP P-2HBA4MP P-2HBA3MP -1.31 1.45 1.31 1.38 -1.31-1.29 Current ,1 0 A -5 Supporting electrolyte Potential, V -1.6 0 1.6 3 -1.2 P-2HBA2AP P-2HBATAP P-2HBA46MP -1.36 1.31 1.03 1.42 -1.45 -1.26 Current ,1 0 A -5
The UV-Vis spectra of the polymers were recorded us-ing MeOH as a solvent, at 25 °C and shown in Fig. 6. Their optical band gaps (Eg) were calculated as in the literature  and shown in Table 4. These results clearly show that the polymers have lower optical band gaps. The optical band gaps (Eg) could be obtained by using the following equation as in the literature :
Eg = 1242 / λonset (4)
where λonset is the onset wavelength which can be de-termined by intersection of two tangents on the absorp-tion edges. λonset also indicates the electronic transition start wavelength. When UV spectra of the polymers in Fig. 6 are considered, the absorption bands at 250– –300 nm may be assigned to π”π* electronic transitions in the aromatic ring and those at 295–380 nm may be as-signed to π”π* electronic transitions in the azomethine group. The bands observed in the UV spectra of the polymers are in the same or close regions, implying that structure of polymers are similar and functional groups (-OH or -CH=N) have the same resonance and inductive effect .
For the polymers, the graph was plotted versus time re-garding to the solid state conductivity values measured at air atmosphere. The measurements for the polymers were
carried out in pure form and then polymers were exposed to iodine vapor in a desiccator, and the change in their con-ductivities versus time was measured at specific time inter-vals by doping. In doping process, electron emitting amine nitrogen and electron pulling iodine coordinate, and the formation of radical cation (polaron) structure in polymer chain (on amine nitrogen) are enabled. The electron vacan-cy formed due to this polaron facilitates the electron flow, which results in an increase in the electrical conductivity. High electron intensity allows the polymer to coordinate with iodine more, and consequently an increase at a higher level for the electron flow is obtained .
Electrical conductivities of the polymers and the chang-es of thchang-ese valuchang-es as a function of doping time with iodine were determined and shown in Fig. 7. Diaz et al.  sug-gested the doping mechanism of Schiff base polymers. According to doping mechanism, nitrogen, being a very electronegative element, is capable of coordinating with an iodine molecule (Scheme E). Consequently, a charge--transfer complex between imine compound and dopant iodine is formed and a considerable increase in conduc-tivity can be observed . However, steric hindrance of the substituents bound with the phenol ring prevents the iodine coordination and consequently could decrease the doping level of the polymer . The experimental results show that a longer doping time is required to ob-tain the maximum conductivity . According to Fig. 7, for poly(azomethine)s, the conductivities of the undoped polymers were 10-10 S·cm-1, after 120 h doping, the con-ductivity of P-2HBA6MP and P-2HBA4MP was found to
T a b l e 4. Electronical structure parameters of the polymers
Compounds HOMOa) eV LUMOb) eV E’gc) eV Egd) eV P-2HBA3MP -5.77 -3.08 2.69 2.52 P-2HBA6MP -5.84 -3.08 2.76 2.49 P-2HBA4MP -5.71 -3.10 2.61 2.50 P-2HBA46MP -5.70 -3.13 2.57 2.49 P-2HBATAP -5.81 -3.03 2.78 2.96 P-2HBA2AP -5.42 -2.94 2.48 2.19
a) Highest occupied molecular orbital; b) lowest unoccupied molecu-lar orbital; c) electrochemical band gap; d) optical band gap.
240 400 600 1 P-2HBA P-2HBA4MP P-2HBA6MP P-2HBA3MP P-2HBATAP P-2HBA46MP P-2HBA2AP 0 Wavelength, nm Absorbance, a.u. -1 -5 2.69 eV 2.61 eV 2.57 eV 2.48 eV 2.78 eV 2.76 eV HOMO HOMO HOMO HOMO HOMO HOMO LUMO LUMO LUMO LUMO LUMO LUMO P-2HBA6M P P-2HBA TAP P-2HBA2A P P-2HBA46M P P-2HBA4M P P-2HBA3M P Ener gy level, eV
Fig. 5. HOMO–LUMO energy levels and electrochemical band gaps of the polymers
Fig. 6. UV-Vis spectra of the polymers
O CH N N CH3 I I I -Scheme E
0 24 48 72 96 120 Doping time, h Conductivity , S /cm 10-10 10-4 P-2HBA P-2HBA46MP P-2HBATAP P-2HBA2AP P-2HBA4MP P-2HBA6MP P-2HBA3MP
Fig. 7. Electrical conductivity changes of the I2-doped at 25 °C
550 350 450 Wavelength, nm Intensity , a.u. P-2HBA6MP P-2HBA P-2HBA2AP P-2HBA46MP P-2HBATAP P-2HBA3MP P-2HBA4MP 1000 0
Fig. 8. Emission spectra of solutions in DMF (slit width:
λEx = 5 nm, λEm = 5 nm; concentration of the compounds:
0.001 g/dm3) 10m 100m 100m 100m 10m 10m 10m 10m 10m
Fig. 9. SEM images of: a) P-2HBA, b) P-2HBA3MP, and c) P-2HBATAP
be around 10-5 S·cm-1 and it is better than the other poly-mers. Poly(azomethine)s showed semiconducting behav-ior, and the conductivity rapidly increased from 10-11 to 10-5 S·cm-1.
A Shimadzu RF-5301PC spectrofluorophotometer was used in the fluorescence measurements. Emission and ex-citation spectra of the polymers were obtained in solu-tion forms in DMF. The measurements were performed at 1 x 10-3 mg/dm3 concentration. Slit width in all measure-ments was 5 nm. The obtained results are also summa-rized in Table 5. According to Table 5 and Fig. 8, out of P-2HBA series poly Schiff bases, P-2HBA3MP has max-imum emission intensity, indicating that it has fluores-cence characteristics while P-2HBA2AP and P-2HBA 46MP have the lowest intensity and display no fluorescence characteristics.
The morphological properties of the polymers were obtained by scanning electron microscopy (FE-SEM) technique. Fig. 9 shows FE-SEM images of surface mor-phologies for P-2HBA, P-2HBA3MP and P-2HBATAP. Ac-cording to Fig. 9 FE-SEM micrographs imply that P-2HBA (a) and P-2HBA3MP (b) have smooth structures in layers but P-2HBATAP (c) has spongy morphology.
Novel polyphenol derivatives of azomethine com-pounds having polyconjugated structures were synthe-sized by oxidative polycondensation reaction. Accord-ing to 1H NMR and 13C NMR spectra, it was found that P-2HBA polymerized via C-O-C or C-C binding, however, polymerization takes place mainly via C-C binding. Mo-lecular mass of P-2HBA2AP was the highest in terms of GPC analysis. Since the other poly Schiff bases contain methylene moieties, binding was less due to steric hin-drance. According to TG and DTA analysis, P-2HBA46MP had the highest thermal stability. Considering DSC analy-sis, ΔCp (thermal capacity) value of P-2HBA3MP was the lowest, implying that amount of energy required to soft-en the polymer was also the lowest. The value of optical band gap (Eg) was in agreement with that of electrochemi-cal band gap electrochemi-calculated by CV (E’g). Furthermore, optical band gap decreased by increasing of conjugation. The low
values of electrochemical and optical band gaps show that the polymers have polyconjugated structure. Conductivi-ties of the polymers are in the range of 10-8–10-11 S·cm-1 and they can be made semiconductor by iodine doping. Con-ductivity measurements clearly indicated that the poly-mers are semiconductor. Compounds containing pyridine and pyrimidine moieties have important applications such as solar cell. Thus, future studies may be on the use of these polymers as solar cell and opto-electronic.
 Adams R., Bullock R.E., Wilson W.C.: Journal of the
American Chemical Society 1923, 45, 521.
 Nishat N., Khan S.A., Rasool R., Parveen S.: Journal
of Inorganic and Organometallic Polymers and Materials
2011, 21, 673.
http://dx.doi.org/10.1007/s10904-011-9457-y  Yıldırım M., Kaya İ.: Polymer 2009, 50, 5653.
http://dx.doi.org/10.1016/j.polymer.2009.06.053  Kaya İ., Aydın A.: Polymers for Advanced Technologies
2009, 21, 337.
 Kaya İ., Yıldırım M., Aydın A., Şenol D.: Reactive and
Functional Polymers 2010, 70, 815.
h t t p : // d x . d o i . o r g / 10 . 10 16 / j . r e a c t f u n c t -polym.2010.07.013
 Mart H., Yürük H., Saçak M. et al.: Polymer
Degrada-tion and Stability 2004, 83, 395.
ht t p://d x.doi.org /10.1016/j.poly mdeg rads -tab.2003.08.003
 Bilici A., Kaya İ., Yıldırım M.: European Polymer
Jour-nal 2011, 47, 1005.
http://dx.doi.org/10.1016/j.eurpolymj.2011.02.019  Kaya İ., Koça S.: Polymer 2004, 45, 1743.
http://dx.doi.org/10.1016/j.polymer.2004.01.035  Doğan F., Kaya İ., Bilici A.: Synthetic Metals 2011, 161,
79. http://dx.doi.org/10.1016/j.synthmet.2010.11.001  Bilici A., Doğan F., Yıldırım M., Kaya İ.: Materials
Chemistry and Physics 2013, 140, 66.
http://dx.doi.org/10.1016/j.matchemphys.2013.02.066  Kaya İ., Vilayetoğlu A.R., Mart H.: Polymer 2001, 42,
4859. http://dx.doi.org/10.1016/S0032-3861(00)00883-1  Kaya İ., Yıldırım M.: Journal of Applied Polymer Science
2007, 106, 2282.
 Kaya İ., Yıldırım M.: European Polymer Journal 2007,
http://dx.doi.org/10.1016/j.eurpolymj.2006.10.014  Colladet K., Nicolas M., Goris L. et al.: Thin Solid Films
2004, 451, 7. http://dx.doi.org/10.1016/j.tsf.2003.10.085  Özbülbül A.: “Synthesis and Characterization of
New Type Oligomer Schiff Bases with Based Oligo-phenol” Master thesis, Institute of Science and Tech-nology, Çukuova University, Adana, Turkey, 2006, p. 108.
T a b l e 5. Fluorescence spectral data of the polymers
Compounds λExa) λ maxEmb) IEmc) P-2HBA 296 345 450 P-2HBA2AP 445 510 25 P-2HBA46MP 305 351 62 P-2HBATAP 277 344 504 P-2HBA3MP 317 348 898 P-2HBA6MP 276 343 411 P-2HBA4MP 316 344 541
a) Excitation wavelength for emission; b) emission wavelength for
 Karakaplan M., Demetgül C., Serin S.: Journal of
Mac-romolecular Science, Part A 2008, 45, 406.
 Erdik E.: “Spectroscopic Methods in Organic Chem-istry”, 5th ed., Gazi Press, Ankara 2008, p. 531.  Çıtakoğlu N.: “Synthesis and Characterization of
Imine Polymers Containing Aliphatic Methylsi-lane Group” Master thesis, Institute of Science and Technology, Çanakkale Onsekiz Mart University, Çanakkale, Turkey, 2012, p. 82.
 Cernini R., Li X-C., Spencer G.W.C. et al.: Synthetic
Metals 1997, 84, 359.
 Cazacu M., Marcu M., Vlad A. et al.: Journal of
Organo-metallic Chemistry 2004, 689, 3005.
http://dx.doi.org/10.1016/j.jorganchem.2004.05.051  Diaz F.R., Moreno J., Tagle L.H. et al.: Synthetic Metals
1999, 100, 187.
http://dx.doi.org/10.1016/S0379-6779(98)01484-2  Kaya İ., Yıldırım M.: Synthetic Metals 2009, 159, 1572.
http://dx.doi.org/10.1016/j.synthmet.2009.04.019  Kaya İ., Yıldırım M.: Journal of Applied Polymer Science
2008, 110, 539.
Received 25 IV 2016.
Politechnika Krakowska i Firma FAMPUR w Bydgoszczyzapraszają do udziału
w Konferencji Naukowo-Technicznej
„Poliuretany 2017 – materiały przyjazne dla człowieka i środowiska”
Ustroń, 8–11 października 2017 r.
• nowe surowce poliolowe i izocyjanianowe • substancje spieniające nowej generacji • katalizatory i inne substancje pomocnicze • nowoczesne rozwiązania technologiczne
• poliuretany wytwarzane metodami bezizocyjanianowymi • modyfikacja kompozycji PUR
• struktura, właściwości, zastosowanie różnych materiałów PUR • zagospodarowanie odpadów
• maszyny i urządzenia do wytwarzania i przetwórstwa PUR • zagadnienia prawne dotyczące przetwórstwa PUR
Patronat medialny: Czasopismo „Polimery”
Miejsce konferencji: Hotel „Muflon”, 43-450 Ustroń, ul. Sanatoryjna 32
Terminy: Zgłoszenie udziału w konferencji z prezentacją oraz przesłanie streszczenia (maks. 100 słów) – 31 marca 2017 r.
Zgłoszenie udziału w konferencji bez prezentacji – 31 lipca 2017 r.
Przesłanie pełnego tekstu wystąpienia do materiałów konferencyjnych – 31 sierpnia 2017 r.
Zgłoszenia oraz teksty i prezentacje do materiałów konferencyjnych należy kierować na firstname.lastname@example.org
lub listownie na adres: Leonard Szczepkowski, FAMPUR Adam Przekurat, ul. Wojciecha Gersona 40/30, 85-305 Bydgoszcz z dopiskiem: Poliuretany 2017.
Uczestnicy z prezentacją: 1000 zł + 23 % VAT (pok. 2–3 os.), 1150 zł + 23 % VAT (pok. 1 os.). Uczestnicy bez prezentacji: 1200 zł + 23 % VAT (pok. 2–3 os.), 1350 zł + 23 % VAT (pok. 1 os.).
Wszyscy uczestnicy po 31 lipca 2017 r.: 1300 zł + 23 % VAT (pok. 2–3 os.), 1450 zł + 23 % VAT (pok. 1 os.). Opłata obejmuje: materiały konferencyjne, noclegi, wyżywienie i udział w imprezach towarzyszących.
Opłatę konferencyjną w odpowiedniej wysokości należy przelać na rachunek: FAMPUR Adam Przekurat, ul. Wojciecha
Gersona 40/30, 85-305 Bydgoszcz, Bank Zachodni WBK S.A. Wrocław; 3 O/Bydgoszcz Nr rachunku: 18 1090 1896 0000 0001 2037 7409